Influence of the Resin Cement Thickness on Bond Strength and Gap Formation of Fiber Posts Bonded to Root Dentin Giovana Mongruel Gomesa / Eluise Cristina de Rezendeb / Osnara Maria Mongruel Gomesc / João Carlos Gomesc / Alessandro Dourado Loguerciod / Alessandra Reise Purpose: To evaluate the effect of the resin cement thickness (RCT) on bond strength (BS) and gap formation (GF) of fiber posts bonded to root dentin. Materials and Methods: The roots of 24 extracted human mandibular premolars were treated endodontically and the post spaces were prepared using drills with different diameters according to the following groups (n = 8): well adapted (WA), moderately well adapted (MA) and poorly adapted (PA). The fiber glass posts were cemented (Excite DSC and Variolink II) in accordance with the manufacturer’s instructions. After 1 week, the roots were transversely sectioned into six 1-mm-thick disks and photographed using an optical microscope to determine the RCT. After this, epoxy resin replicas of each sample were observed using SEM, and the mean length and width of the gaps formed in the cement/dentin/post interface were measured. Finally, each sample was subjected to the push-out test (0.5 mm/min), and the data were statistically analyzed using one-way ANOVA and Tukey’s tests at the 5% level of significance. Results: The lowest RCT (μm) was observed for WA and the highest for PA. The group MA showed an intermediate value. Significantly higher push-out BS values were observed for WA compared to the other groups. The MA and PA groups were statistically similar. The highest mean gap length (%) and width (μm) were observed for PA. The groups MA and WA were statistically similar. Conclusion: Lower resin cement thickness resulted in better fiber post adhesion, that is, in higher bond strength and less gap formation. Keywords: bond strength, fiber posts, gap, resin cements, root dentin, scanning electron microscopy. J Adhes Dent 2014; 16: 71–78. doi: 10.3290/j.jad.a30878
eeth with considerable loss of dental structure often require endodontic treatment, and in the majority of cases, this leads to the use of intraradicular retainers and filling cores to retain the final restoration.49 a
Dentist, PhD Student, Department of Restorative Dentistry, School of Dentistry, State University of Ponta Grossa, Ponta Grossa, Paraná, Brazil. Idea/ hypothesis, designed and performed experiments, collected data, wrote and edited manuscript as partial fulfillment of PhD degree.
Dentist, PhD Student, Department of Microbiology, School of Dentistry, State University of Ponta Grossa, Ponta Grossa, Paraná, Brazil. Performed all endodontic treatments, co-wrote manuscript.
Professor, Department of Restorative Dentistry, School of Dentistry, State University of Ponta Grossa, Ponta Grossa, Paraná, Brazil. Idea, designed experiments, co-wrote manuscript.
Professor, Department of Restorative Dentistry, School of Dentistry, State University of Ponta Grossa, Ponta Grossa, Paraná, Brazil. Analyzed data, cowrote manuscript, and contributed substantially to discussion.
Professor, Department of Restorative Dentistry, School of Dentistry, State University of Ponta Grossa, Ponta Grossa, Paraná, Brazil. Idea/hypothesis, designed experiments, analyzed data, co-wrote and edited manuscript.
Correspondence: Giovana Mongruel Gomes, Universidade Estadual de Ponta Grossa, St Carlos Cavalcanti 4748, Uvaranas, Ponta Grosa, Paraná, Brazil 84030-900. Tel: +55-423-222-6560, Fax: +55-423-224-7351. e-mail: [email protected]
Vol 16, No 1, 2014
Submitted for publication: 29.08.12; accepted for publication: 27.04.13
Moreover, to restore these teeth, an attractive option has been to use materials with a modulus of elasticity similar to that of dentin,4,8,24,32 resulting in biomimetics between the properties of dentin and the post/cement set.42 This favors a more uniform stress distribution in the root structure,21,33,38 which reduces the risk of root fractures. In spite of the advantages of using these glass fiber posts, they are prefabricated and therefore do not always adapt closely to the root canal. There are root canals that exhibit extensive tissue destruction due to carious lesions, previous restoration with excessive post and core diameters, endodontic over-instrumentation, incomplete physiological root development due to traumatic impacts, internal resorption, developmental anomalies, or even oval-shaped root canals.5,29 In these cases, the remaining root structure is thin, which probably weakens it, even when a glass fiber post is cemented in place.50 Clinical situations of this nature make the restorative procedure difficult, and the long-term clinical prognosis of these teeth is still unknown. Thus, the restoration of weakened roots presents a challenge to dentists. 71
Gomes et al
The treatment of highly widened root canals using prefabricated posts may not provide ideal conditions for root canal fillings, thereby obliging the operator to employ excessive quantities of cement to replace lost structure.22 The deformation resulting from polymerization shrinkage when thick layers of cement are used may cause greater polymerization stress at the cement/dentin and cement/ post interfaces, inducing structural discontinuities, such as bubbles, spaces, or gaps, which in turn weaken the retention of posts to root canals.20 Prospective and retrospective clinical studies have indicated that fiber post displacement occurs with greater frequency with thicker cement layers.13,15 Although some clinical alternatives have been described in the literature, eg, the use of accessory fiber posts27 and the restoration of weakened roots with composite resins and glass fiber posts,50 the ideal thickness of resin cement for cementation of glass fiber posts is still unknown. Few studies have evaluated the effect of the size discrepancy between root canal openings and fiber post diameter on bond strength (BS) and gap formation at the cement/dentin interfaces, and their results are conflicting.10,31 Therefore, the aim of this study was to evaluate the effect of resin cement thickness (RCT) on BS between the glass fiber post and root dentin and gap formation (GF) at the cement/dentin and cement/post interfaces, mediated by conventional dual-curing resin cement. Two null hypotheses were tested: 1. there are no differences in the push-out BS to dentin for different RCTs between the fiber post and root walls, and 2. there are no differences in GF at the adhesive interfaces for different RCTs between the fiber post and root walls.
MATERIALS AND METHODS This research project was approved by the Research Ethics Committee of the School of Dentistry, State University of Ponta Grossa, report number 25/2011 and protocol number 18741/10. Twenty-four extracted human mandibular premolars were stored in distilled water at 4°C and used within 6 months after extraction (ISO/TS 11405).23 The inclusion criteria included the following: absence of caries or root cracks; absence of prior endodontic treatments, posts, or crowns; absence of severe root curvatures; a root length of 14 ± 1 mm as measured from the cementoenamel junction (CEJ). Endodontic Treatment Teeth were cross-sectioned immediately below the CEJ using a low-speed diamond saw (Isomet 1000, Buehler; Lake Bluff, IL, USA). Endodontic access was made using a bur with a high-speed handpiece and water spray. Working length was established by inserting a #10 Flexofile (Dentsply Maillefer; Petrópolis, RJ, Brazil) into each canal until it was visible at the apical foramen. The working length was determined by subtracting 72
1 mm from the canal length. A crown-down technique was used for instrumentation with Gates Glidden drills #2 to #4 (Dentsply Maillefer). Apical enlargement was performed to size 40 and 0.06 taper. Irrigation was performed after every change of instrument by alternating 1 ml of 1% NaOCl solution and 17% EDTA solution. Roots were dried with paper points (Dentsply Maillefer; Petrópolis, RJ, Brazil), filled with resin-based sealer (AH Plus, Dentsply DeTrey; Konstanz, Germany) and guttapercha points using the warm vertical condensation technique. The root access was provisionally filled with conventional glass-ionomer cement (Vitro Fil, DFL; Rio de Janeiro, RJ, Brazil). The roots were stored at 37°C in 100% humidity for a week. Post Space Preparation and Experimental Groups After one week, the roots were randomly divided into 3 groups (n = 8) according to the preparation of the post space: WA: well adapted (low RCT); MA: moderately welladapted (medium RCT); PA: poorly adapted (high RCT). For this purpose, the post spaces were prepared with drills of different diameters. In the WA and MA groups, the post spaces were prepared with a low-speed drill provided by the post manufacturer (Whitepost DC, FGM; Joinville, Santa Catarina, Brazil). In WA, a drill corresponding to the #0.5 post was used, which had the same crown diameter as the post (1.4 mm), and in MA, the drill corresponding to the # 3 post with a 2.0-mm crown diameter was used. In PA, the post spaces were prepared with a conical diamond bur # 4137 (KG Sorensen; Barueri, São Paulo, Brazil) with a 2.6-mm crown diameter adapted at a low speed. A conical diamond bur was used in this group because there is no other commercially available post drill with a greater crown diameter. However, after root canal widening with the diamond bur, the drill corresponding to the #0.5 post was used in order to standardize the smear layer in the root dentin. In all groups, the same brand of fiber glass post (cylindrical with tapered end [Whitepost DC # 0.5, FGM]) with a crown diameter of 1.4 mm was cemented. The working length was 10 mm for all teeth, respecting the limit of the apical 4 mm of endodontic filling material. One bur was used for only 6 preparations. After the post space preparations, the canals were irrigated with 10 ml of distilled water and dried with paper points. To ensure that there was no residual gutta-percha on the walls after post space preparation, a radiographic evaluation of each root was performed. Post Luting Procedures Before the cementation procedures, each fiber glass post was horizontally sectioned with a water-cooled diamond rotary cutting instrument so that a total length of 13 mm remained. Ten mm of the post length were cemented inside the root canal, while the remaining cervical 3 mm served as a guide to standardize the distance of the light-curing device from the cervical root area. The root canal walls were etched with 37% phosphoric acid gel (Total-Etch, Ivoclar Vivadent; Schaan, Liechtenstein). The gel was introduced into the canal through a The Journal of Adhesive Dentistry
Gomes et al
needle and washed after 15 s with an endodontic syringe. Excess water was removed from the post space by gently blowing air into it and using paper points, leaving the dentin slightly moist. After this, a specific microbrush (Excite DSC Endo microbrush, Ivoclar Vivadent) was used to apply two coats of the dual-curing two-step etch-andrinse adhesive (Excite DSC, Ivoclar Vivadent) to the root canal. A paper point was used to absorb the excess adhesive solution. The base and catalyst components of the resin cement (Variolink II, Ivoclar Vivadent) were then mixed, and the resin cement was introduced into the root canal space with a Centrix syringe28 (DFL) before seating the fiber post. After the fiber post was seated, the excess resin cement was removed, and the remaining cement was light polymerized through the post for 40 s with an LED light-curing device (L.E. Demetron I/ Kerr; Orange, CA, USA) using a power density of 800 mW/cm2. After the post luting procedures, the roots with cemented posts were covered with conventional glass-ionomer cement (Vitro Fil, DFL), and all samples were stored in water at 37°C for 1 week. Sample Preparation Subsequently, the roots were placed in separate polyvinyl chloride (PVC) tubes and embedded in acrylic resin (Duralay, Reliance Dental; Alsip, IL, USA). The portion of each root that contained the bonded fiber post was sectioned perpendicular to the long axis into six 1-mm-thick slices. An Isomet 1000 saw (Buehler) was used under water cooling to create two cervical, two middle, and two apical slices. Then, all specimens were observed with a light stereomicroscope at 10X magnification in order to identify any artifacts caused by the sectioning procedure. If any defects were observed, the slices were discarded. Resin Cement Thickness (RCT) All of the slices were photographed with an optical microscope (Olympus model BX 51; Tokyo, Japan) at 100X magnification. Each photograph was marked with an “X” that divided it into 4 segments, and measurements were taken perpendicular to the lines forming the “X”. For each sample (slice), four measurements were taken at the 4 endpoints of the “X”. The mean RCT (μm) of each sample (slice) was calculated for statistical purposes. The RCT was measured using the UTHSCSA ImageTool 3.0 software (Department of Dental Diagnostic Science, University of Texas Health Science Center, San Antonio, Texas, USA). SEM Evaluation of Cement/Dentin Interfacial Gap Three slices of each tooth, one from each root third, were randomly selected for evaluating gap formation. Impressions of the slice surfaces were taken with addition silicone (Virtual, Ivoclar Vivadent) in order to create positive replicas in epoxy resin (Alpha Resiqualy; Curitiba, Brazil). Each replica was mounted on a metal stub and sputter coated with 200 Å of gold-palladium in a Polaron SC7620 “Mini” sputter coater (Quorum Technologies; East Sussex, UK) for 5 min at a current of 10 mA. After Vol 16, No 1, 2014
this, each specimen was examined using SEM (JSM 6360LV, JEOL; Tokyo, Japan) at different magnifications (30X to 2000X) using 15 kV accelerating voltage. Measurements were made of the entire length and width of the gaps, using UTHSCSA ImageTool 3.0 software. In each slice, the widest gap at the cement/dentin interface was measured (μm) by two different, calibrated operators. The length of the gap was expressed as a percentage of the total length of the bonded area. In both measurements, the values taken from the 3 slices from the same tooth were averaged for statistical purposes. If any disagreement occurred during evaluation, a consensus was obtained. Each slice was also categorized as either having or lacking bubbles/voids within the resin cement layer. This procedure was also performed by two evaluators who needed to reach a consensus in case of disagreements. Push-out Test The coronal side of each slice was identified, and its thickness was measured with a Mitutoyo digital caliper (Kyoto, Japan) with an accuracy of 0.01 mm. The slices were also photographed on both sides with an optical microscope (Olympus, model BX 51) at 40X magnification in order to calculate the coronal and apical diameters of the posts with the purpose of calculating their individual bonding areas. This measurement was also taken with the UTHSCSA ImageTool 3.0 software. Each specimen (slice) was subjected to a push-out BS test using a universal loading device (AG-I, Shimadzu Autograph; Tokyo, Japan) at a crosshead speed of 0.5 mm/ min. The load was applied in the apical-coronal direction until the post was dislodged. Care was taken to center the push-out pin on the center of the post surface without stressing the surrounding post space walls. With regard to the tapered design of the post, different sizes of punch pins were used which matched the diameter of the post at the different root thirds being tested. The maximum failure load was recorded in Newtons (N) and converted into MPa by dividing the applied load by the bonded area. Two bonded areas were used for the calculation of the BS: the lateral surface of the fiber post area and the lateral surface of the root canal. For both calculations, the bonded area was the lateral surface of a truncated cone, and it was calculated by using the formula: LS = π(R + r)[(h2 + (R – r)2]0.5 where π = 3.14, R = coronal post radius or root canal radius (coronal post + resin cement radius), r = apical post radius or apical root canal radius (post + resin cement radius), and h = root slice thickness. Failure Mode Analysis After push-out evaluation, the failure modes of all specimens were evaluated under a stereomicroscope (40X magnification). Each debonded specimen was analyzed by two independent, calibrated operators. The failure modes were classified according to the following criteria: 73
Gomes et al
Table 1 Means and standard deviations of resin cement thickness (μm), gap length (%), and gap width (μm) for the experimental groups Experimental groups
Resin cement thickness (μm)
Gap length (%)
Gap width (μm)
1.4 ± 1.8a 4.1 ± 3.9a
75.2 ± 17.9a
Well adapted Moderately well adapted
341.9 ± 8.5b
17.0 ± 13.4a
628.9 ± 24.4c
45.5 ± 9.3b
35.5 ± 9.9b
Comparisons are valid only for columns. Similar lowercase superscript letters indicate statistically similar means (p > 0.05).
Ce 43.1 μm
Ce 6.2 μm
Ce 500 μm
Fig 1 Scanning electron micrographs of representative resin cement thickness (double arrow in a, c, and e) and gap widths (line in d and f) formed in the cement/dentin interface for each group (a,b: well adapted; c,d: moderately well adapted; e,f: poorly adapted). No gaps were found in b (well adapted). Abbreviations: De = dentin; Po = post; Ce = cement.
1. adhesive failure between dentin and luting cement; 2. adhesive failure between luting cement and post; 3. cohesive failure within luting cement; 4. cohesive failure within the post; 5. cohesive failure within dentin; 6. mixed failure. If any disagreement occurred between the evaluators, a consensus had to be obtained. Statistical Analysis The experimental unit for all properties evaluated was the root; therefore, all values obtained for a single root were averaged for statistical purposes. The data obtained for RCT, BS, length, and width of the gaps were statistically analyzed using one-way ANOVA and Tukey’s test for pairwise comparisons at a 5% level of significance. The two approaches used for the BS calculation were compared by paired t-tests at a 5% level of significance. 74
The percentage of slices with bubbles/voids were evaluated using the chi-square test (_ = 0.05). Correlations between the RCT and BS, RCT and mean gap length, RCT and mean gap width, BS and mean gap length, and BS and mean gap width were evaluated using the Pearson product moment correlation test (_ = 0.05). Pairwise comparisons of the failure modes were analyzed by utilizing Fisher’s exact test (_ = 0.05). Sigma Plot 11 software (Systat Software; San Jose, CA, USA) was used for these calculations.
RESULTS None of the specimens presented artifacts caused by the sectioning procedure; therefore, none were discarded. One-way ANOVA detected significant differences in the RCT (p < 0.001). The lowest RCT (μm) values were observed for WA, while the highest were observed for PA. MA showed an intermediate RCT value (Table 1). The Journal of Adhesive Dentistry
Gomes et al
Table 2 Means and standard deviations of push-out bond strength (MPa) for the experimental groups using the different methods for calculation of the bonded area Experimental Groups
Bond strength (MPa) Post radius
Root canal radius
23.3 ± 2.8aA
20.2 ± 2.2aA
Moderately well adapted
17.1 ± 3.9bA
10.0 ± 2.0bB
15.8 ± 3.2bA
7.3 ± 1.4cB
Lowercase superscript letters indicate the comparisons within each column. Uppercase superscript letters indicate the comparison within each row. Identical letters indicate statistically similar means (p > 0.05).
Distribution of the failure mode among the different experimental groups
Cohesive in cement
Cohesive in post
Cohesive in dentin
Moderately well adapted
No cohesive failures in cement, post and dentin or adhesive failures between cement and the post were observed. Significantly more mixed failures occurred for all the groups.
As regards gap evaluation, statistical analysis revealed significant differences in the mean gap length and width (p < 0.0001). The highest mean gap length (%) and width (μm) were observed for the PA. The groups MA and WA were statistically similar (Table 1). A representative image of the RCT and gap widths for each group can be seen in Fig 1. From the total of 24 slices evaluated in each group, 10 (42%), 14 (58%), and 24 (100%) for groups WA, MA, and PA, respectively, showed gaps (chi-square test, p = 0.0001). Similarly, 14 (58%), 19 (79%), and 24 (100%) for groups WA, MA, and PA, respectively, showed the presence of bubbles/voids within the resin cement (chi-square test, p = 0.002). The use of the post radius for the calculation of BS resulted in higher values than the use of the root canal radius (Table 2). Significant differences in BS values were detected by one-way ANOVA, considering the post radius (p = 0.006) as well as the root canal radius (p < 0.0001). Higher push-out BS values were observed for WA irrespective of how the BS was calculated (Table 2). MA and PA were statistically similar (p > 0.05) when the post radius was used for BS calculation; however, they differed when root canal radius was used (Table 2). The analysis of the failure mode is shown in Table 3. No cohesive fracture in cement, post, and dentin or adhesive failure between the cement and post were observed in this study. Significantly more mixed failures occurred for all of the groups (p < 0.02), and no significant difference in the fracture pattern was observed among them (p > 0.05). Vol 16, No 1, 2014
The Pearson product moment correlation test showed a moderate, negative, significant correlation between RCT and BS (r = -0.665; p = 0.0003). A strong, positive, significant correlation between the RCT and mean gap length (r = 0.8274; p < 0.0001) and RCT and mean gap width (r = 0.8396; p < 0.0001) was also detected (Fig 2). For all correlation tests, the BS values calculated using the post radius were employed. A moderate, negative, significant correlation between BS and mean gap length (r = -0.4676; p = 0.0184) was observed, whereas a negative but non-significant correlation between BS and mean gap width (r = -0.3718; p = 0.0671) was detected (Fig 2).
DISCUSSION Most of the studies that evaluate the bonding of fiber posts to root canals calculate the bond strength based on the lateral area of the fiber post.11,17-19,25,31,35,45,46 However, this study demonstrated that this procedure overestimated the BS values, because debonding does not occur at the interface between the resin cement and the fiber post, but rather, between the cement and the root canal walls. Thus, it seems that the use of the lateral area of the root canal is the best method for the calculation of BS, as has been similarly done in a few previous studies.26,43 The present study detected that all of the specimens from the PA group showed gap formation at the interface 75
y = 0.013x+23.35 R2 = 0.442 R = –0.665 P = 0.0003
Mean gap length (%)
Push-out bond strength (MPa)
Gomes et al
15 10 5 0 0
y = 0.068x–0.500 R2 = 0.684 R = 0.8274 P < 0.0001
60 50 40 39 20 10 0 0
Mean gap length (%)
Mean gap width (μm)
40 30 20 10 0 –10 0
y = 0.062x–7.919 R2 = 0.705 R = 0.8396 P < 0.0001
Resin cement thickness (μm)
Resin cement thickness (μm)
y = –1.907x+58.94 R2 = 0.218 R = –0.4676 P = 0.0184
60 50 40 30 20 10 0
Resin cement thickness (μm)
Push-out bond strength (MPa)
Mean gap width (μm)
60 y = –1.354x+38.96 R2 = 0.138 R = –0.3718 P = 0.0671
50 40 30 20 10 0 0
Push-out bond strength (MPa)
and bubbles/voids within the resin cement. Even in the well-adapted specimens, a gap-free interface was not observed. This means that obtaining perfect adhesion and the creation of a perfect monoblock system between the post, resin cement, dentin is an unrealistic expectation,41 one that cannot be accomplished in a clinical scenario. The high C-factor of the closed cavity in root canals (close to 200) led to higher polymerization stress, resulting in gaps at the adhesive interface,7,41 even under ideal conditions of adaptation. It is known that an adverse chemical interaction between unpolymerized acidic monomers (oxygen inhibition layer of the simplified adhesive) and the tertiary amine from the auto/dual-curing composite may occur.36,40 This might 76
Fig 2 Significant linear correlations between the properties evaluated in this study.
also have favored gap formation at the adhesive interface, as the two-step etch-and-rinse adhesive system (Excite DSC) was used with the dual-curing resin cement (Variolink II). Moreover, two-step etch-and-rinse systems have been shown to function as permeable membranes,39,40 allowing water movement across their structure even after polymerization,6,9 which may adversely affect the bond of auto/ dual-curing resin cements to the dentin surface.9,39 However, the present study showed that the magnitude of gap formation and the resultant BS within the adhesive interface was dependent on the fiber post adaptation to the root canal, which led us to reject both the first and second null hypotheses. According to Feilzer et al,12 the composite sample thickness affects stress The Journal of Adhesive Dentistry
Gomes et al
distribution. This is accentuated in thin layers due to increased boundary restraints (C-factor), contributing to an inverse relationship between film thickness and shrinkage stress.2,3 However, although this means that a higher stress contraction is expected to occur under WA, some authors have shown that if the bond strength values to the tooth structure were sufficiently high, thin adhesive joints might enhance the bond strength of luted restorations.1 Additionally, as demonstrated in the current study, thicker RCT contains more structural discontinuities, such as bubbles, cracks, or gaps; these are expected to produce stress concentration zones.20 These zones are responsible for starting the fracture line and therefore reducing the BS of the fiber post to the root canals, as observed in the present investigation. It should be borne in mind that the appearance of bubbles and voids is also dependent on the cement application method.28,47,48 For instance, it was demonstrated that the use of a flexible root canal-shaped application aid, such as an elongation tip,47,48 a Lentulo drill or Centrix syringe,28 to insert the resin cement into the root canal improved the homogeneity of the resin cement layer. In the present study, the resin cement was introduced into the root canal space with a Centrix syringe. Another important aspect to be considered in the poorly adapted specimens is that the increased amount of resin cement could have adversely affected the absorption of light and, hence, the polymerization reaction of the resin cement within its entire thickness. It is possible that sufficient light transmission did not occur through the post to adequately light polymerize the entire RCT in the MA and PA groups. Thus, the polymerization of resin cement in thicker layers may have relied only on the chemical activation produced by the self-curing component of the dual polymerization system. This resulted in the formation of resin cement with reduced mechanical properties as well as lower BS to the root canal. Indeed, it has been demonstrated that dual-curing resin cements that polymerize only by chemical activation do not reach levels of hardness as high as those polymerized under dual conditions (light and chemical activation).14 Based on these findings, it can be assumed that the RCT could be a determining factor in the clinical performance of FRC posts. This finding seems to predispose the restoration to debonding, as observed earlier in prospective and retrospective clinical studies.13,15 The positive, significant correlation between gap length/width and RCT suggests that the increase in RCT significantly decreases the bonding integrity and BS of fiber posts to the root canals. However, to the extent of the authors’ knowledge, the relationship between RCT and gap formation has not been investigated prior to this study. On the other hand, the relationship between RCT and BS was examined in earlier studies, which produced conflicting results.10,30,31,37 While the results of the present study are in agreement with the study by Schmage et al,37 other authors10,30,31 did not find any correlation between RCT and post retention or BS. Vol 16, No 1, 2014
This lack of consensus suggests that other factors besides the degree of mismatch between the fiber post and the root canals may play a role in BS. This may lead one to speculate that either the resin cement itself or the adhesive system might have been the weak link at the adhesive interfaces; therefore, the effect of RCT was minor and not detected in the previous studies.10,30,31 The fact that laboratory studies16,35,43 reported low BS values when testing the resin cement used in the Perez et al31 study strengthens this hypothesis. Additionally, the adhesive system employed by Perdigão et al30 has shown poor performance in clinical studies.34,44 The present study has some limitations, for instance, the test specimen crowns were not totally restored, and no thermal cycling or mechanical stress was applied. These factors may limit the direct application of the study results to clinical conditions. Another limitation is that only one resin cement and adhesive system were employed to investigate the research question. As resin cements and adhesive systems differ in their chemical and mechanical properties, caution should be used when applying the results of the present study to other materials available on the market. This study showed that the fitting of the fiber post to the root canal may be a clinical problem, and alternative methods should be studied to avoid such issues, which would thereby reduce the RCT under clinical conditions in order to minimize gap formation and maximize fiber post retention in root canals.
CONCLUSIONS Within the limitations of this in vitro study, it was demonstrated that the push-out bond strength of fiber posts in oversized dowel spaces cemented with the tested resin cement decreased significantly when compared with that of precisely fitting posts, most likely due to increased gap formation. It is advisable to prepare post spaces that allow for the chosen fiber post to fit into the space as accurately as possible.
ACKNOWLEDGMENTS The authors are very grateful to Dr. Eng. Milton Domingos Michel for his support in performing the SEM analysis, to the undergraduate student Felipe Auer Trentini for his support with the resin cement thickness measurements, and to Ivoclar Vivadent and FGM for the donation of the cementation system and fiber posts used in this study. This study was partially supported by the National Council for Scientific and Technological Development (CNPq) grants 301937/2009-5 and 301891/2010-9. Part of the funding for this study was obtained from a productivity scholarship provided by the “Fundação Araucária”.
Gomes et al
4. 5. 6.
12. 13. 14.
23. 24. 25.
Alster D, Feilzer AJ, De Gee AJ, Davidson CL. Tensile strength of thin resin composite layers as a function of layer thickness. J Dent Res 1995;74:1745-1748. Alster D, Feilzer AJ, de Gee AJ, Davidson CL. Polymerization contraction stress in thin resin layers as a function of layer thickness. Dent Mater 1997;13:146-150. Alster D, Venhoven BAM, Feilzer AJ, Davidson CL. Influence of compliance of the substrate materials on polymerization contraction stress in thin resin layers. Biomaterials 1997;18:337-341. Asmussen E, Peutzfeldt A, Heitmann T. Stiffness, elastic limit, and strength of newer types of endodontic posts. J Dent 1999;27:275-278. Baba NZ, Goodacre CJ, Daher T. Restoration of endodontically treated teeth: the seven keys to success. Gen Dent 2009;57:596-603. Bonfante EA, Pegoraro LF, de Goes MF, Carvalho RM. SEM observation of the bond integrity of fiber-reinforced composite posts cemented into root canals. Dent Mater 2008;24:483-491. Bouillaguet S, Troesch S, Wataha JC, Krejci I, Meyer JM, Pashley DH. Microtensile bond strength between adhesive cements and root canal dentin. Dent Mater 2003;19:199-205. Braem M, Lambrechts P, Van Doren V, Vanherle G. The impact of composite structure on its elastic response. J Dent Res 1986;65:648-653. Chersoni S, Acquaviva GL, Prati C, Ferrari M, Grandini S, Pashley DH, Tay FR. In vivo fluid movement through dentin adhesives in endodontically treated teeth. J Dent Res 2005;84:223-227. D’Arcangelo C, Cinelli M, De Angelis F, D’Amario M. The effect of resin cement film thickness on the pullout strength of a fiber-reinforced post system. J Prosthet Dent 2007;98:193-198. D‘Arcangelo C, D‘Amario M, Vadini M, Zazzeroni S, De Angelis F, Caputi S. An evaluation of luting agent application technique effect on fibre post retention. J Dent 2008;36:235-240. Feilzer AJ, de Gee AJ, Davidson CL. Increased wall-to-wall curing contraction in thin bonded resin layers. J Dent Res 1989;68:48-50. Ferrari M, Vichi A, Mannocci F, Mason PN. Retrospective study of the clinical performance of fiber posts. Am J Dent 2000;13:9B-13B. Fonseca RG, Cruz CA, Adabo GL. The influence of chemical activation on hardness of dual-curing resin cements. Braz Oral Res 2004;18: 228-232. Fredriksson M, Astbäck J, Pamenius M, Arvidson K. A retrospective study of 236 patients with teeth restored by carbon fiber-reinforced epoxy resin posts. J Prosthet Dent 1998;80:151-157. Galhano G, de Melo RM, Valandro LF, Bottino MA. Comparison of resin push-out strength to root dentin of bovine- and human-teeth. Indian J Dent 2009;20:332-336. Giachetti L, Grandini S, Calamai P, Fantini G, Russo DS. Translucent fiber post cementation using light- and dual-curing adhesive techniques and a self-adhesive material: push-out test. J Dent 2009;37:638-642. Gomes GM, Gomes OM, Reis A, Gomes JC, Loguercio AD, Calixto AL. Regional bond strengths to root canal dentin of fiber posts luted with three cementation systems. Braz Dent J 2011;22:460-467. Goracci C, Tavares AU, Fabianelli A, Monticelli F, Raffaelli O, Cardoso PC, Tay F, Ferrari M. The adhesion between fiber posts and root canal walls: comparison between microtensile and push-out bond strength measurements. Eur J Oral Sci 2004;112:353–361. Grandini S, Goracci C, Monticelli F, Borracchini A, Ferrari M. SEM evaluation of the cement layer thickness after luting two different posts. J Adhes Dent 2005;7:235-240. Hayashi M, Ebisu S. Key factors in achieving firm adhesion in post-core restorations. Jap Dent Sci Rev 2008;44:22-28. Hornbrook DS, Hastings JH. Use of bondable reinforcement fiber for post and core build-up in an endodontically treated tooth: maximizing strength and aesthetics. Pract Periodontics Aesthet Dent 1995;7:33-42. International Standardization for Organization. Guidance on testing of adhesion to tooth structure. Geneve, Switzerland: 2003, CD TR 11405. Lassila LV, Tanner J, Le Bell AM, Narva K, Vallittu PK. Flexural properties of fiber reinforced root canals posts. Dent Mater 2004;20:29-36. Manicardi CA, Versiani MA, Saquy PC, Pécora JD, de Sousa-Neto MD. Influence of filling materials on the bonding interface of thin-walled roots reinforced with resin and quartz fiber posts. J Endod 2011; 37:531-537. Marques de Melo R, Bottino MA, Galvão RK, Soboyejo WO. Bond strengths, degree of conversion of the cement and molecular structure of the adhesive-dentine joint in fibre post restorations. J Dent 2012;40:286-294.
27. Martelli H Jr, Pellizzer EP, Rosa BT, Lopes MB, Gonini A Jr. Fracture resistance of structurally compromised root filled bovine teeth restored with accessory glass fibre posts. Int Endod J 2008;41:685-692. 28. Michida SM, Souza RO, Bottino MA, Valandro LF. Cementation of fiber post: influence of the cement insertion techniques on the bond strength of the fiber post-root dentin and the quality of the cement layer. Minerva Stomatol 2010;59:633-636. 29. Morgano SM, Rodrigues AH, Sabrosa CE. Restoration of endodontically treated teeth. Dent Clin North Am 2004;48:397-416. 30. Perdigão J, Gomes G, Augusto V. The effect of dowel space on the bond strengths of fiber posts. J Prosthodont 2007;16:154-164. 31. Perez BE, Barbosa SH, Melo RM, Zamboni SC, Özcan M, Valandro LF, Bottino MA. Does the thickness of the resin cement affect the bond strength of a fiber post to the root dentin? Int J Prosthodont 2006;19:606-609. 32. Peutzfeldt A, Asmussen E. Modulus of resilience as predictor for clinical wear of restorative resins. Dent Mater 1992;8:146-148. 33. Qualtrough AJ, Manocci F. Tooth-colored post systems: a review. Oper Dent 2003;28:86-91. 34. Reis A, Loguercio AD. A 36-month clinical evaluation of ethanol/water and acetone-based etch-and-rinse adhesives in non-carious cervical lesions. Oper Dent 2009;34:384-391. 35. Sadek FT, Goracci C, Monticelli F, Grandini S, Cury AH, Tay F, Ferrari M. Immediate and 24-hour evaluation of the interfacial strengths of fiber posts. J Endod 2006;32:1174-1177. 36. Sanares AM, Itthagarun A, King NM, Tay FR, Pashley DH. Adverse surface interactions between one-bottle light-cured adhesives and chemical-cured composites. Dent Mater 2001;17:542-556. 37. Schmage P, Pfeiffer P, Pinto E, Platzer U, Nergiz I. Influence of oversized dowel space preparation on the bond strengths of FRC posts. Oper Dent 2009;34:93-101. 38. Schmitter M, Rammelsberg P, Lenz J, Scheuber S, Schweizerhof K, Rues S. Teeth restored using fiber-reinforced posts: in vitro fracture tests and finite element analysis. Acta Biomat 2010;6:3747-3754. 39. Tay FR, Pashley DH, Suh BI, Carvalho RM, Itthagarun A. Single-step adhesives are permeable membranes. J Dent 2002;30:371-382. 40. Tay FR, Pashley DH, Yiu CK, Sanares AM, Wei SH. Factors contributing to the incompatibility between simplified-step adhesives and chemicallycured or dual-cured composites. Part I. Single-step self-etching adhesive. J Adhes Dent 2003;5:27-40. 41. Tay FR, Loushine RJ, Lambrechts P, Weller RN, Pashley DH. Geometric factors affecting dentin bonding in root canals: a theoretical modeling approach. J Endod 2005;31:584-589. 42. Tay FR, Pashley DH. Monoblocks in root canals: a hypothetical or a tangible goal. J Endod 2007;33:391-398. 43. Valandro LF, Baldissara P, Galhano GA, Melo RM, Mallmann A, Scotti R, Bottino MA. Effect of mechanical cycling on the push-out bond strength of fiber posts adhesively bonded to human root dentin. Oper Dent 2007;32:579-588. 44. van Dijken JW. Clinical evaluation of three adhesive systems in class V non-carious lesions. Dent Mater 2000;16:285-291. 45. Vano M, Cury AH, Goracci C, Chieffi N, Gabriele M, Tay FR, Ferrari M. Retention of fiber posts cemented at different time intervals in canals obturated using an epoxy resin sealer. J Dent 2008;36:801-807. 46. Wang VJ, Chen YM, Yip KH, Smales RJ, Meng QF, Chen L. Effect of two fiber post types and two luting cement systems on regional post retention using the push-out test. Dent Mater 2008;24:372-377. 47. Watzke R, Blunck U, Frankenberger R, Naumann M. Interface homogeneity of adhesively luted glass fiber posts. Dent Mater 2008;24: 1512-1517. 48. Watzke R, Frankenberger R, Naumann M. Probability of interface imperfections within SEM cross-sections of adhesively luted GFP. Dent Mater 2009;25:1256-1263. 49. Zicari F, Couthino E, De Munck J, Poitevin A, Scotti R, Naert I, van Meerbeek B. Bonding effectiveness and sealing ability of fiber-post bonding. Dent Mater 2008;24:967-977. 50. Zogheib LV, Pereira JR, do Valle AL, de Oliveira JA, Pegoraro LF. Fracture resistance of weakened roots restored with composite resin and glass fiber post. Braz Dent J 2008;19:329-33.
Clinical relevance: Fiber posts that fit accurately in the root canal possess higher bond strength and less gap formation than posts with inaccurate fit.
The Journal of Adhesive Dentistry